LMucko/crystallography-open-database huggingface dataset:
Structural redetermination of the Th Ni phase
Fornasini, M.L.; Acta Crystallographica C (39,1983-) 39 (1983) 946–947; doi:

data_2020033
_publ_section_title
;
 Structural redetermination of the Th Ni phase
;
_journal_name_full               'Acta Crystallographica C (39,1983-)'
_journal_page_first              946
_journal_page_last               947
_journal_volume                  39
_journal_year                    1983
_chemical_formula_sum            'Ni Th'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   14.146
_cell_length_b                   4.286
_cell_length_c                   5.702
_cell_volume                     345.711
_citation_journal_id_ASTM        ACSCEE
_cod_data_source_file            Fornasini_ACSCEE_1983_1531.cif
_cod_data_source_block           Ni1Th1
_cod_original_cell_volume        345.7108
_cod_original_formula_sum        'Ni1 Th1'
_cod_database_code               2020033
Structures of Ba8 Ga7, Sr8 Ga7 and Sr8 Al7
Fornasini, M.L.; Acta Crystallographica C (39,1983-) 39 (1983) 943–946; doi:

data_2020034
_publ_section_title
;
 Structures of Ba8 Ga7, Sr8 Ga7 and Sr8 Al7
;
_journal_name_full               'Acta Crystallographica C (39,1983-)'
_journal_page_first              943
_journal_page_last               946
_journal_volume                  39
_journal_year                    1983
_chemical_formula_sum            'Ga7 Sr8'
_space_group_IT_number           198
_symmetry_space_group_name_Hall  'P 2ac 2ab 3'
_symmetry_space_group_name_H-M   'P 21 3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.484
_cell_length_b                   12.484
_cell_length_c                   12.484
_cell_volume                     1945.635
_citation_journal_id_ASTM        ACSCEE
_cod_data_source_file            Fornasini_ACSCEE_1983_361.cif
_cod_data_source_block           Ga7Sr8
_cod_database_code               2020034
Gd Mg5: a complex structure with a large cubic cell
Fornasini, M.L.; Manfrinetti, P.; Gschneidner, K.A.jr.; Acta Crystallographica C (39,1983-) 42 (1986) 138–141; doi:

data_2020035
_publ_section_title
;
 Gd Mg5: a complex structure with a large cubic cell
;
_journal_name_full               'Acta Crystallographica C (39,1983-)'
_journal_page_first              138
_journal_page_last               141
_journal_volume                  42
_journal_year                    1986
_chemical_formula_sum            'Gd9.08 Mg45.9'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   22.344
_cell_length_b                   22.344
_cell_length_c                   22.344
_cell_volume                     11155.339
_citation_journal_id_ASTM        ACSCEE
_cod_data_source_file            Fornasini_ACSCEE_1986_439.cif
_cod_data_source_block           Gd9.08Mg45.9
_cod_original_cell_volume        11155.34
_cod_database_code               2020035
Die Struktur des Na7 Ga13 - I und ein Konzept zur bindungs- maessigen Deutung
Frank-Cordier, U.; Cordier, G.; Schaefer, H.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (33,1978-41,1986) 37 (1982) 119–126; doi:

data_7221111
_publ_section_title
;
 Die Struktur des Na7 Ga13 - I und ein Konzept zur bindungs- maessigen
 Deutung
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (33,1978-41,1986)
;
_journal_page_first              119
_journal_page_last               126
_journal_volume                  37
_journal_year                    1982
_chemical_formula_sum            'Ga13 Na7'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            18
_cell_length_a                   14.965
_cell_length_b                   14.965
_cell_length_c                   38.93
_cell_volume                     7550.374
_citation_journal_id_ASTM        ZNBAD2
_cod_data_source_file            Frank-Cordier_ZNBAD2_1982_229.cif
_cod_data_source_block           Ga13Na7
_cod_original_cell_volume        7550.375
_cod_database_code               7221111
Die Struktur des Na7 Ga13 - I und ein Konzept zur bindungs- maessigen Deutung
Frank-Cordier, U.; Cordier, G.; Schaefer, H.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (33,1978-41,1986) 37 (1982) 119–126; doi:

data_7221112
_publ_section_title
;
 Die Struktur des Na7 Ga13 - I und ein Konzept zur bindungs- maessigen
 Deutung
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (33,1978-41,1986)
;
_journal_page_first              119
_journal_page_last               126
_journal_volume                  37
_journal_year                    1982
_chemical_formula_sum            'Ga4 Na'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.23
_cell_length_b                   4.23
_cell_length_c                   11.272
_cell_volume                     201.689
_citation_journal_id_ASTM        ZNBAD2
_cod_data_source_file            Frank-Cordier_ZNBAD2_1982_230.cif
_cod_data_source_block           Ga4Na1
_cod_original_cell_volume        201.6888
_cod_original_formula_sum        'Ga4 Na1'
_cod_database_code               7221112
Neue Ga-Cluster-Verbaende im Na7 Ga13 - II
Frank-Cordier, U.; Cordier, G.; Schaefer, H.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (33,1978-41,1986) 37 (1982) 127–135; doi:

data_7221113
_publ_section_title
;
 Neue Ga-Cluster-Verbaende im Na7 Ga13 - II
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (33,1978-41,1986)
;
_journal_page_first              127
_journal_page_last               135
_journal_volume                  37
_journal_year                    1982
_chemical_formula_sum            'Ga13 Na7'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   15.625
_cell_length_b                   14.979
_cell_length_c                   21.678
_cell_volume                     5073.668
_citation_journal_id_ASTM        ZNBAD2
_cod_data_source_file            Frank-Cordier_ZNBAD2_1982_231.cif
_cod_data_source_block           Ga13Na7
_cod_database_code               7221113
Die Struktur der Phase Li5 Sn2
Frank, U.; Mueller, W.; Schaefer, H.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (2,1947-32,1977) 30 (1975) 1–5; doi:

data_7221114
_publ_section_title
;
 Die Struktur der Phase Li5 Sn2
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (2,1947-32,1977)
;
_journal_page_first              1
_journal_page_last               5
_journal_volume                  30
_journal_year                    1975
_chemical_formula_sum            'Li5 Sn2'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   4.74
_cell_length_b                   4.74
_cell_length_c                   19.83
_cell_volume                     385.842
_citation_journal_id_ASTM        ZENBAX
_cod_data_source_file            Frank_ZENBAX_1975_1003.cif
_cod_data_source_block           Li5Sn2
_cod_original_cell_volume        385.8424
_cod_database_code               7221114
Die Kristallstruktur der Phase Li7 Sn2
Frank, U.; Mueller, W.; Schaefer, H.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (2,1947-32,1977) 30 (1975) 6–9; doi:

data_7221115
_publ_section_title
;
 Die Kristallstruktur der Phase Li7 Sn2
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (2,1947-32,1977)
;
_journal_page_first              6
_journal_page_last               9
_journal_volume                  30
_journal_year                    1975
_chemical_formula_sum            'Li7 Sn2'
_space_group_IT_number           65
_symmetry_space_group_name_Hall  '-C 2 2'
_symmetry_space_group_name_H-M   'C m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.8
_cell_length_b                   13.8
_cell_length_c                   4.75
_cell_volume                     642.390
_citation_journal_id_ASTM        ZENBAX
_cod_data_source_file            Frank_ZENBAX_1975_1004.cif
_cod_data_source_block           Li7Sn2
_cod_original_cell_volume        642.39
_cod_database_code               7221115
Darstellung und Struktur der Phase Li13 Sn5
Frank, U.; Mueller, W.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (2,1947-32,1977) 30 (1975) 316–322; doi:

data_7221116
_publ_section_title
;
 Darstellung und Struktur der Phase Li13 Sn5
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (2,1947-32,1977)
;
_journal_page_first              316
_journal_page_last               322
_journal_volume                  30
_journal_year                    1975
_chemical_formula_sum            'Li13 Sn5'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   4.7
_cell_length_b                   4.7
_cell_length_c                   17.12
_cell_volume                     327.514
_citation_journal_id_ASTM        ZENBAX
_cod_data_source_file            Frank_ZENBAX_1975_1006.cif
_cod_data_source_block           Li13Sn5
_cod_original_cell_volume        327.5142
_cod_database_code               7221116
The crystal structure of Mn2 Hg5
de Wet, J.F.; Acta Crystallographica (1,1948-23,1967) 14 (1961) 733–738; doi:

data_2310198
_publ_section_title
;
 The crystal structure of Mn2 Hg5
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              733
_journal_page_last               738
_journal_volume                  14
_journal_year                    1961
_chemical_formula_sum            'Hg5 Mn2'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.7577
_cell_length_b                   9.7577
_cell_length_c                   2.998
_cell_volume                     285.448
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            deWet_ACCRA9_1961_641.cif
_cod_data_source_block           Hg5Mn2
_cod_original_cell_volume        285.4477
_cod_database_code               2310198
Phase Transition in Hydrogen-Bonded 1-Adamantane-methanol
Hassine, Bacem Ben; Negrier, Philippe; Barrio, María; Mondieig, Denise; Massip, Stéphane; Tamarit, Josep Ll.; Crystal Growth & Design 15 (2015) 4149–; doi:10.1021/acs.cgd.5b00764

data_4513378
_publ_section_title
;
 Phase Transition in Hydrogen-Bonded 1-Adamantane-methanol
;
_journal_issue                   8
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              4149
_journal_paper_doi               10.1021/acs.cgd.5b00764
_journal_volume                  15
_journal_year                    2015
_chemical_formula_sum            'C11 H18 O'
_chemical_formula_weight         166.25
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_audit_creation_date             2015-05-29
_audit_creation_method           'Materials Studio'
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.518(5)
_cell_angle_gamma                90.0000
_cell_formula_units_Z            12
_cell_length_a                   13.0675(7)
_cell_length_b                   11.2831(8)
_cell_length_c                   19.3721(14)
_cell_measurement_temperature    90(1)
_cell_volume                     2856.1(3)
_diffrn_ambient_temperature      90(1)
_diffrn_measurement_device_type  'Inel CPS120'
_diffrn_radiation_monochromator  'curved quartz'
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a~1~
_diffrn_radiation_wavelength     1.540562
_exptl_crystal_density_diffrn    1.160
_exptl_crystal_description       'Powder Sample'
_cod_data_source_file            cg5b00764_si_002.cif
_cod_data_source_block           'global_AdaMet90K'
_cod_depositor_comments          'Adding full bibliography for 4513378.cif.'
_cod_original_sg_symbol_H-M      P21/N
_cod_database_code               4513378
The pressure-induced transformation B1 to B2 in actinide compounds
Gerward, L.; Olsen, J.S.; Dabos-Seignon, S.; Benedict, U.; Steenstrup, S.; Journal of Applied Crystallography 23 (1990) 515–519; doi:

data_2300514
_publ_section_title
;
 The pressure-induced transformation B1 to B2 in actinide compounds
;
_journal_name_full               'Journal of Applied Crystallography'
_journal_page_first              515
_journal_page_last               519
_journal_volume                  23
_journal_year                    1990
_chemical_formula_sum            'Te U'
_chemical_name_systematic        'U Te'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.765
_cell_length_b                   3.765
_cell_length_c                   3.765
_cell_volume                     53.370
_citation_journal_id_ASTM        JACGAR
_cod_data_source_file            Gerward_JACGAR_1990_525.cif
_cod_data_source_block           Te1U1
_cod_original_cell_volume        53.36973
_cod_original_formula_sum        'Te1 U1'
_cod_database_code               2300514
New intermediate phases in systems of Nb or Ta with Rh, Ir, Pd, or Pt
Giessen, B.C.; Grant, N.J.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 615–616; doi:

data_2310199
_publ_section_title
;
 New intermediate phases in systems of Nb or Ta with Rh, Ir, Pd, or Pt
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              615
_journal_page_last               616
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Nb Pd3'
_space_group_IT_number           59
_symmetry_space_group_name_Hall  'P 2 2ab -1ab'
_symmetry_space_group_name_H-M   'P m m n :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            6
_cell_length_a                   5.486
_cell_length_b                   13.602
_cell_length_c                   4.845
_cell_volume                     361.537
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Giessen_ACCRA9_1964_1363.cif
_cod_data_source_block           Nb1Pd3
_cod_original_cell_volume        361.5367
_cod_original_sg_symbol_Hall     '-P 2ab 2a (x-1/4,y-1/4,z)'
_cod_original_formula_sum        'Nb1 Pd3'
_cod_database_code               2310199
New intermediate phases in systems of Nb or Ta with Rh, Ir, Pd, or Pt
Giessen, B.C.; Grant, N.J.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 615–616; doi:

data_2310200
_publ_section_title
;
 New intermediate phases in systems of Nb or Ta with Rh, Ir, Pd, or Pt
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              615
_journal_page_last               616
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Nb Pt3'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.53
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   27.33
_cell_length_b                   5.537
_cell_length_c                   4.87
_cell_volume                     736.927
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Giessen_ACCRA9_1964_1370.cif
_cod_data_source_block           Nb1Pt3
_cod_original_cell_volume        736.9271
_cod_original_formula_sum        'Nb1 Pt3'
_cod_database_code               2310200
New intermediate phases in systems of Nb or Ta with Rh, Ir, Pd, or Pt
Giessen, B.C.; Grant, N.J.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 615–616; doi:

data_2310201
_publ_section_title
;
 New intermediate phases in systems of Nb or Ta with Rh, Ir, Pd, or Pt
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              615
_journal_page_last               616
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Nb0.2 Pt0.8'
_chemical_name_systematic        '(Nb0.2 Pt0.8)'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.94
_cell_length_b                   3.94
_cell_length_c                   3.94
_cell_volume                     61.163
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Giessen_ACCRA9_1964_1371.cif
_cod_data_source_block           Nb0.2Pt0.8
_cod_original_cell_volume        61.16299
_cod_database_code               2310201
New intermediate phases in systems of Nb or Ta with Rh, Ir, Pd, or Pt
Giessen, B.C.; Grant, N.J.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 615–616; doi:

data_2310202
_publ_section_title
;
 New intermediate phases in systems of Nb or Ta with Rh, Ir, Pd, or Pt
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              615
_journal_page_last               616
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Nb Rh'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   2.842
_cell_length_b                   2.842
_cell_length_c                   3.809
_cell_volume                     30.765
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Giessen_ACCRA9_1964_1380.cif
_cod_data_source_block           Nb1Rh1
_cod_original_cell_volume        30.76516
_cod_original_formula_sum        'Nb1 Rh1'
_cod_database_code               2310202
New intermediate phases in transition metal systems. II
Giessen, B.C.; Grant, N.J.; Acta Crystallographica (1,1948-23,1967) 18 (1965) 1080–1081; doi:

data_2310203
_publ_section_title
;
 New intermediate phases in transition metal systems. II
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              1080
_journal_page_last               1081
_journal_volume                  18
_journal_year                    1965
_chemical_formula_sum            'Pd1.5 Ru1.5 Ta'
_chemical_name_systematic        '(Pd0.5 Ru0.5)3 Ta'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.893
_cell_length_b                   3.893
_cell_length_c                   3.893
_cell_volume                     59.000
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Giessen_ACCRA9_1965_1732.cif
_cod_data_source_block           Pd1.5Ru1.5Ta1
_cod_original_cell_volume        59.00016
_cod_original_formula_sum        'Pd1.5 Ru1.5 Ta1'
_cod_database_code               2310203
New intermediate phases in transition metal systems. II
Giessen, B.C.; Grant, N.J.; Acta Crystallographica (1,1948-23,1967) 18 (1965) 1080–1081; doi:

data_2310204
_publ_section_title
;
 New intermediate phases in transition metal systems. II
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              1080
_journal_page_last               1081
_journal_volume                  18
_journal_year                    1965
_chemical_formula_sum            'Pd2.16 Rh0.84 Ta'
_chemical_name_systematic        '(Pd0.72 Rh0.28)3 Ta'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            9
_cell_length_a                   5.517
_cell_length_b                   5.517
_cell_length_c                   20.26
_cell_volume                     534.043
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Giessen_ACCRA9_1965_1736.cif
_cod_data_source_block           Pd2.16Rh0.84Ta1
_cod_original_cell_volume        534.0428
_cod_original_formula_sum        'Pd2.16 Rh0.84 Ta1'
_cod_database_code               2310204
New intermediate phases in transition metal systems. II
Giessen, B.C.; Grant, N.J.; Acta Crystallographica (1,1948-23,1967) 18 (1965) 1080–1081; doi:

data_2310205
_publ_section_title
;
 New intermediate phases in transition metal systems. II
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              1080
_journal_page_last               1081
_journal_volume                  18
_journal_year                    1965
_chemical_formula_sum            'Pd2.01 Rh0.99 Ta'
_chemical_name_systematic        '(Pd0.67 Rh0.33)3 Ta'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            10
_cell_length_a                   5.52
_cell_length_b                   5.52
_cell_length_c                   22.43
_cell_volume                     591.886
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Giessen_ACCRA9_1965_1737.cif
_cod_data_source_block           Pd2.01Rh0.99Ta1
_cod_original_formula_sum        'Pd2.01 Rh0.99 Ta1'
_cod_database_code               2310205